OPEN

The topological Anderson insulator phase in the Kane-Mele model Christoph P. Orth1, Tibor Sekera1, Christoph Bruder1 & Thomas L. Schmidt2

received: 24 December 2015 accepted: 09 March 2016 Published: 05 April 2016

It has been proposed that adding disorder to a topologically trivial mercury telluride/cadmium telluride (HgTe/CdTe) quantum well can induce a transition to a topologically nontrivial state. The resulting state was termed topological Anderson insulator and was found in computer simulations of the BernevigHughes-Zhang model. Here, we show that the topological Anderson insulator is a more universal phenomenon and also appears in the Kane-Mele model of topological insulators on a honeycomb lattice. We numerically investigate the interplay of the relevant parameters, and establish the parameter range in which the topological Anderson insulator exists. A staggered sublattice potential turns out to be a necessary condition for the transition to the topological Anderson insulator. For weak enough disorder, a calculation based on the lowest-order Born approximation reproduces quantitatively the numerical data. Our results thus considerably increase the number of candidate materials for the topological Anderson insulator phase. Topological insulators (TIs) are novel materials which have raised a great deal of interest over the past decade1,2. One of their distinguishing features is the existence of conducting boundary states together with an insulating bulk. The boundary states are protected by time-reversal symmetry (TRS) and exist both in two-dimensional (2D) and three-dimensional (3D) TIs. In 2D TIs, the boundary states lead to an edge conductance of one conductance quantum per edge for chemical potentials inside the bulk band gap3–5. It is a challenging task to find candidate materials for TIs. So far, only a limited number of materials are known. The most prominent 2D TIs are HgTe/(Hg, Cd)Te quantum wells (HgTeQWs)6 and InAs/GaSb heterostructures7,8, whereas 3D TIs were found for instance in Bi1−xSbx9. The fact that their metallic surface states emerge due to a topological property of the bulk band structure means that they are robust to weak disorder. However, one expects that a large amount of disorder should ultimately localize the surface states and render them insulating. All the more surprising, it was predicted that the opposite transition can happen in certain parameter ranges: adding strong disorder can convert a trivial insulator without edge states into a topological insulator with perfectly conducting edge states. Materials that exhibit this new state have been termed topological Anderson insulators (TAIs). This effect was first theoretically predicted based on the lattice version of the Bernevig-Hughes-Zhang (BHZ) model for HgTeQWs in the presence of Anderson disorder10,11. For Anderson disorder, a random on-site potential, uniformly distributed in an energy window of width 2W, is assigned to each lattice site of a tight-binding model. From Anderson’s theory of localization12 one expects that a system with finite conductance without disorder undergoes a transition to a system with localized states and suppressed conductance as the disorder is increased beyond a certain threshold value. The behavior of TAIs instead is quite different. A TAI is an ordinary band insulator in the clean limit. Above a critical disorder strength W, an interesting topological state appears, in which the material features a quantized conductance. For even stronger W, above the disorder strength at which the states of the conduction and valence band localize, it was proposed that tunneling across the bulk becomes possible13, probably enabled by percolating states14, and the conductance is again suppressed. The disorder-induced transition can be understood by a renormalization of the model parameters. The BHZ model with disorder and band mass m can be approximated by an effective model of a clean system and renormalized mass m ¯ . Using an effective-medium theory and the self-consistent Born approximation (SCBA), it was shown that for certain model parameters, m ¯ can become negative even if the bare mass m is positive15. As a consequence, the effective model becomes that of a TI and features edge states with a quantized conductance of G0 = e2/h16.

1 Department of Physics, University of Basel, Klingelbergstrasse 82, 4056 Basel, Switzerland. 2Physics and Materials Science Research Unit, University of Luxembourg, L-1511 Luxembourg. Correspondence and requests for materials should be addressed to C.P.O. (email: [email protected])

Scientific Reports | 6:24007 | DOI: 10.1038/srep24007

1

www.nature.com/scientificreports/ Furthermore, TAIs have been predicted in several related systems, for instance in a honeycomb lattice described by the time-reversal-symmetry breaking Haldane model17, a modified Dirac model17, the BHZ model with sz non-conserving spin-orbit coupling18, as well as in 3D topological insulators19. Moreover, similar transitions from a topologically trivial to a topologically nontrivial phase have been found to be generated by periodically varying potentials20 or phonons21. In contrast to on-site Anderson disorder, certain kinds of bond disorder cannot produce a TAI as they lead only to a positive correction to m22,23. So far, however, the TAI phase was not found in the Kane-Mele model on a honeycomb lattice, describing for example graphene or proposed TIs such as silicene, germanene and stanene24–27. First indications to this phase were already found, showing that the Kane-Mele model without a staggered sublattice potential hosts extended bulk states even for large disorder strengths28. In this paper we show the existence of TAIs in the Kane-Mele model by means of tight-binding calculations. The interplay between the parameters characterizing intrinsic spin-orbit coupling (SOC) λSO, extrinsic Rashba SOC λR, and a staggered sublattice potential λν turns out to be crucial for the visibility of TAIs, and we calculate the parameter ranges in which TAIs can be observed. We find analytically that to lowest order in W, the parameters λSO and λR are not renormalized with increasing disorder strength, in contrast to λν. However, a new effective hopping λR3 is generated due to the disorder, which is related but not identical to λR. Although λR is not a crucial ingredient for the existence of TAIs, it significantly alters the physics of topological insulators in various ways29,30 and, as we will show below, strongly affects the TAI state. Even though recently first signs of a TAI phase may have been found experimentally in evanescently coupled waveguides31, there has been no experimental evidence so far for the existence of the TAI phase in fermionic systems. The main difficulty is the requirement of a rather large and specific amount of disorder, which is difficult to control in the topological insulators currently investigated, where the 2D TI layer is buried inside a semiconductor structure. In contrast, producing and controlling disorder in 2D materials described by the Kane-Mele model could be much easier. Disorder in 2D materials with honeycomb structure can be produced by randomly placed adatoms32,33 or a judicious choice of substrate material34–37. Moreover, a sizeable staggered sublattice potential can be generated via a suitable substrate material38. Other means of engineering disorder were proposed in periodically driven systems39,40. Finally, honeycomb structures with the SOC necessary to produce a topological phase have already been realized using ultracold atoms in optical lattices41, in which disorder can in principle be engineered.

Results

Setup. The basis of our calculations is the Kane-Mele model5 given by the following Hamiltonian on a tight-binding honeycomb lattice H = t ∑ci† c j + iλSO ∑ ν ij ci† s zc j + λ ν ∑ξ i ci† c i ij

i

ij

+ iλ R ∑ ij

ci† (s

× dˆ ij ) c j + W ∑i ci† c i , z

i

(1)

which has been supplemented by an on-site Anderson disorder term with disorder strength W and uniformly distributed random variables i ∈ [ − 1, 1]. The summations over the lattice sites 〈 ij〉 and 〈 〈 i, j〉 〉 include all nearest neighbors and next-nearest neighbors, respectively. The operators ci† = (ci†↑, ci†↓ ), c i = (c i ↑, c i ↓)T are creation and annihilation operators for the site i of the lattice. The parameters t, λSO and λR are the nearest-neighbor hopping strength, intrinsic SOC, and Rashba SOC, respectively. If the next-nearest neighbor hopping from site j to site i corresponds to a right-turn on the honeycomb lattice, then ν ij = 1, otherwise ν ij = −1. Furthermore, s = (sx, sy, sz) is the vector of Pauli matrices for the spin degree of freedom, and dˆ ij is the unit vector between sites j and i. The Wannier states at the two basis atoms of the honeycomb lattice are separated in energy by twice the staggered sublattice potential λν, with ξi = 1 for the A sublattice and ξi = −1 for the B sublattice. The lattice constant is a. The band structure of this model depends strongly on the parameter set λSO, λR, and λν. In the clean limit and for λR = 0, the system will be a topological insulator for λν /λSO3 3 λSO > λ¯ ν . The system thus makes a transition from a trivial insulator to a topological insulator with increasing W. For a more quantitative treatment, we evaluate the integral for the full Hamiltonian (k ) numerically. The self-energy ∑ is then written as a linear combination of several independent contributions Σ=

5

5

a =0

a